- Nano Express
- Open Access
Two novel hierarchical homogeneous nanoarchitectures of TiO2 nanorods branched and P25-coated TiO2 nanotube arrays and their photocurrent performances
Nanoscale Research Lettersvolume 6, Article number: 91 (2011)
We report here for the first time the synthesis of two novel hierarchical homogeneous nanoarchitectures of TiO2 nanorods branched TiO2 nanotube arrays (BTs) and P25-coated TiO2 nanotube arrays (PCTs) using two-step method including electrochemical anodization and hydrothermal modification process. Then the photocurrent densities versus applied potentials of BTs, PCTs, and pure TiO2 nanotube arrays (TNTAs) were investigated as well. Interestingly, at -0.11 V and under the same illumination condition, the photocurrent densities of BTs and PCTs show more than 1.5 and 1 times higher than that of pure TNTAs, respectively, which can be mainly attributed to significant improvement of the light-absorbing and charge-harvesting efficiency resulting from both larger and rougher surface areas of BTs and PCTs. Furthermore, these dramatic improvements suggest that BTs and PCTs will achieve better photoelectric conversion efficiency and become the promising candidates for applications in DSSCs, sensors, and photocatalysis.
In current years, one-dimensional (1D) TiO2 nanostructure materials, especially nanotubular [1–3] and hierarchical [4–7] nanoarchitecture TiO2 nanotube arrays (TNTAs), have initiated increasing research interest owing to their intriguing architectures because they possess very high specific surface areas and a dual-channel for the benefit of the electrons transportation from interfaces to electrodes [7–13]. These nanostructure materials have shown very promising applications in dye-sensitized solar cells (DSSCs) [14–16], photocatalysis [17–19], photosplitting water [20, 21], sensors [22, 23], photoelectrochemical cells , and piezoelectronics . However, as far as we are concerned, tremendous efforts have been conducted to improve the geometrical factors of the nanotube layers [8–13, 26], to convert amorphous TiO2 nanotubes into different crystalline forms (i.e., anatase or rutile phase, or mixture phases of anatase and rutile) through high temperature annealing for high performance applications [27–29], and also many studies have devoted one's mind to change the crystal structure or chemistry composition of the tubes by modifying and doping [30–33]. There still remain many challenges to prepare and discuss the homogeneous modification of TNTAs, although the similar synthesis method of growing branched ZnO nanowires  and the decoration process of growing TiO2 nanoparticles on TiO2 nanotubes by a TiCl4 treatment  have been reported. Therefore, it is particularly valuable to seek some facile and high-efficiency method to synthesize the modification of TNTAs nanostructures for further specific surface area.
In this communication, we report for the first time the synthesis of two novel hierarchical homogeneous modification nanoarchitectures (i.e., P25-coated TNTAs, PCTs; and TiO2 nanorods branched TNTAs, BTs) via two-step method of electrochemical anodization and hydrothermal modification approach. The main precursors of modification are the P25 (Degussa, Germany) and titanium(IV) isopropoxide (TTIP of 95%). Erenow, the optimized nanoarchitecture TNTAs (with bigger pore diameter, longer length, and larger space among tubes) have been prepared by electrochemical anodization method. Interestingly, the as-synthesized BTs and PCTs with beautiful morphologies show both larger and rougher surface area, and these properties result in dramatic improvement of light-absorbing and charge-harvesting efficiency, which has been shown through the UV-Vis diffuse reflectance spectroscopic spectra and photoelectrochemical performances in this article.
Fabrication of optimum nanoarchitecture TNTAs
In this article, TNTAs were prepared using a typical anodization approach . Briefly, the fabrication process of the optimum nanoarchitecture TNTAs with bigger pore diameter, larger space among tubes and longer length was described as follows, Titanium foil samples, about 200 μm × 2 cm × 3.5 cm (Purity≥99.6%, from ShengXin non-ferrous metal Co., LTD, Baoji, Shanxi, China) were cleaned with soap, acetone, and iso-propanol before anodization. A two-electrode configuration was used for anodization, with Ti foil as the anode, and platinum foil as the cathode. A 99.7% pure Ti foil (0.2 mm thickness, 2 × 3 cm2) was immersed in the electrolyte containing 0.35 wt% NH4F (85% Lactic Acid) and 10 vol.% DMSO (dimethyl sulphoxide: purity ≥99.0%) at a 45 V constant potential for 9 h. Thus we obtained the amorphous TNTAs, and then the as-prepared TNTAs were annealed at 400°C for 1.5 h for further use.
Synthesis of hierarchical homogeneous nanoarchitecture BTs
The BTs were obtained via a modification process of growing TiO2 nanorods on the as-prepared TNTAs by conventional hydrothermal growth method. Briefly, the as-prepared TNTAs were immersed in a beaker with growth solution, this solution was consisted of 90 mL of 0.8 M HCl (36-38%) with constant stirring at 25°C for about 15 min. After that, 6 mL of TTIP of 95% as precursor was dropped (0.16 μL/s) in mixture solution, kept stirring for 1 h [7, 32, 33], and then the beaker was sealed and heated at 95°C for 9 h, with slight stirring maintained for the entire heating process to grow TiO2 nanorods on the TNTAs. After the reaction, the reactant was cooled freely to room temperature and washed several times with ethanol and distilled water, and the as-prepared BTs were obtained. The BTs were finally achieved through annealing in a muffle furnace at 400°C for 2 h.
Fabrication of hierarchical homogeneous nanoarchitecture PCTs
We fabricated PCTs via a hydrothermal approach of coating P25 on the as-prepared TNTAs. About 0.4 g P25 (Degussa, Germany) was put into a beaker with 300 mL of distilled water, then they were mixed through vigorous magnetic stirring and ultrasonicating alternately at room temperature more than 5 times (about 10 min per time), After that, the mixed solution was kept state static more than 3 h, and then transferred into a Teflon-lined autoclave (80 mL), in which the as-prepared TNTAs were suspended. The autoclave was sealed and heated at 80-120°C for 12 h to coat P25 on the TNTAs, and then it was cooled freely to room temperature and washed several times with distilled water, thus the as-prepared PCTs were obtained. Finally, the PCTs were fabricated after the as-prepared PCTs were annealed at 400°C for 2 h.
The crystal structures of the as-synthesized samples were firstly determined by using a Bruker D8 advance X-ray diffractometer (XRD, Cu Kα radiation; λ = 1.5418 Å). Then the morphologies were observed by field-emission scanning electron microscopy (FESEM, JOEL, JSM-6700F), and transmission electron microscopy (TEM and HRTEM, JEM-2010FEF; 200 kV). Photoelectrochemical experiments were carried out using a three-electrode configuration (CH instruments, CHI 660C) with a Pt wire counter electrode, a reference saturated calomel electrode and a working electrode. The all samples used as working electrodes were illuminated with a 150~350 W adjustable xenon lamp (from Shanghai Lansheng Electronics Co., LTD., Model, XQ350W). The measured light irradiance was approximately 100 mW/cm2, and the scan rate was 100 mV/s
Results and discussion
In this study, the two-step method is used to synthesize the BTs and PCTs. The first step is the fabrication of the optimize nanoarchitecture TNTAs [36, 37]. From Figure 1, it can be found that the TNTAs show very nice highly ordered, self-organized, and free-standing morphologies, and the optimize geometrical architectures (average external diameter, 350 nm; tube length, 3.5 μm; wall thickness, 10 nm; and space among tubes, 60 nm), and also show at least local single-crystalline status. These characterizations can be observed from the FESEM images of the top view and cross-section of the TNTAs shown in Figure 1a and the TEM, SAED, and HRTEM images in Figure 1b.
The second step is the synthesis of BTs and PCTs using hydrothermal modification method. In brief, they were obtained from growing branched TiO2 nanorods and coating P25 on the pre-prepared TNTAs via hydrothermal modification process, the images of obtained BTs and PCTs are shown in Figures 2 and 3, respectively. As for the BTs, the mechanism of the formation of TiO2 crystal nucleus and growth of the anisotropic 1D nanocrystalline TiO2 nanorods, and their corresponding FESEM images are depicted in Figure 4. From schematic diagram of the morphologies evolution of the BTs and the FESEM images, it is clearly observed that more and more TiO2 nanocrystal nucleus were firstly formed on the rough surfaces of the TiO2 tubes with special bamboo structures, many rings and attached particles, these special structures and morphologies are the probable cause of crystal nucleus formed. And then the nucleus gradually grew up and became increasing TiO2 nanorods along the backbones of the TiO2 tubes, along with a small quantity of free-grown rods random adhered to the backbones of the tubes. Thus these TiO2 nanorods made BTs have both larger and rougher surface area [7, 34]. Furthermore, the same conclusion can also be confirmed by the top view FESEM images showed in Figure 2a, c, the cross-sectional view in Figure 2b, the TEM image of a individual branched TiO2 nanotube in Figure 2d. And the insets in Figure 2d are the SAED pattern and the HRTEM images, which show the BTs are evident polycrystalline.
Figure 3 is the characterization of another homogeneity nanostructure (the PCTs). Figure 3a is the top view FESEM image of the PCTs. A cross-sectional view in Figure 3b shows that the length of the tubes is the same as that of TNTAs (about 3.5 μm) and the P25 nanoparticles are densely grown on the whole surface (including inside and outside) of the TiO2 tubes. And the top view of the PCTs with many attached P25 particles is clearly shown by the high-magnification FESEM image in Figure 3c. Meanwhile, Figure 3d shows the PCTs' TEM image, and its inset of the HRTEM image shows the (101) crystal facet and the 0.35 nm interplane distance of a typical anatase TiO2 while the another inset of the SAED pattern shows that the PCTs are polycrystalline structure . The growth mechanism of the PCTs is mainly dependent on the special structures and morphology of TNTAs, especially its bigger pore diameter, larger space among tubes, and rough surface. Moreover, annealing plays an important role in the process of transforming the P25 on the TiO2 tube surface from attached state into crystallization state.
Otherwise, the X-ray diffraction (XRD) patterns in Figure 5a, b, c are also employed to characterize the properties of the obtained samples. We can find that the diffraction peaks of the samples (b, c) and the dominant diffraction peaks of the samples (a) match well with the crystal structure of the anatase TiO2 phase (JCPDS 21-1272)  except for one peak of the Ti (101). The main reason can be attributed to thermal treatment temperature of no more than 400°C for 2 h. It is noteworthy that the two peaks [R (110) and R (211)] in Figure 5a just match with the crystal structure of the rutile TiO2 nanorod (JCPDS no. 21-1276) [7, 12], this comes from those rutile TiO2 nanorods grown on the TNTAs.
On the basis of the above observations and structural analyses, we conclude that both of the BTs and PCTs can provide larger and rougher surface areas than the TNTAs compared with the arrays of same geometrical size and quantity [7, 34, 35]. As a result, this larger and rougher surface areas are favorable to improve light-absorbing and charge-harvesting efficiency and to absorb more dye for better photoelectric conversion efficiency and better applications such as photocatalysis, sensors, etc. Moreover, it is also found that the growth length and density of the TiO2 nanorods of the BTs can be readily controlled by adjusting the growth time and the concentration of growth solution, and that the density of the coated P25 particles can also be controlled through changing the coating time and the concentration of coating solution.
Figure 6 shows the UV-Vis diffuse reflectance spectra of three samples (TNTAs, PCTs, and BTs) and Ti foil. Comparing to the UV-Vis absorption spectrum of the TNTAs, the absorption edges of the samples (PCTs and BTs) displayed appreciable shifts (BTs is a little bit larger than PCTs) to visible region revealing some decreases in their band gaps. This conclusion is mainly consistent with the above discussions and the previous studies [39–41]. Simultaneously, it can also be found that the absorption intensity of each sample (TNTAs, PCTs, and BTs) is gradually increasing after their absorption peaks. The cause for this effect mainly comes from absorption effect of the annealed (400°C, 2 h) Ti foil substrate to visible (see the inset in Figure 6). Otherwise, the general UV-Vis absorption spectra only reflect the intrinsic optical property for the bulk of a solid. However, the actual absorption spectrum of a photocatalyst is an overlapping result of intrinsic and extrinsic absorption bands .
Furthermore, Figure 7 clearly shows the comparison curves of the photocurrent densities versus applied potentials for three different TiO2 photoanodes (TNTAs, BTs, and PCTs) under Xe lamp irradiation (100 mW/cm2) in 1 M KOH electrolyte . It can be observed that the values of the photocurrent densities of BTs and PCTs are dramatically greater than that of TNTAs. At -0.11 V and under the same illumination conditions, the photocurrent density of BTs shows more than 1.5 times higher than that of TNTAs while PCTs versus TNTAs is more than 1 times higher. These experimental results are well consistent with the effect from above UV-Vis diffuse reflectance spectra. They suggest that the BTs and PCTs used as photoanodes can harvest more solar light and more photogenerated charge than that of the TNTAs with the same geometrical structure. In addition, the photocurrent densities of the BTs and PCTs also show a steeper increase when their applied potentials are over -0.7 V. Thus as for the BTs and PCTs, e--h+ pairs induced by photon absorption are split more readily compared with the TNTAs. The conclusion mainly results from the fact that more incident photons are absorbed on the electrode with larger and rougher space area .
In summary, we have reported here the fabrication of two novel hierarchical homogeneous nanoarchitectures of BTs and PCTs with larger and rougher surface areas via facile hydrothermal modification process. Based on the investigation of the photocurrent densities versus applied potential, the photocurrent density of BTs, at -0.11 V and under the same illumination conditions, shows more than 1.5 times higher than that of TNTAs while PCTs versus TNTAs is more than 1 times higher. On the basis of the results and discussion, we conclude that the dramatically improved photocurrent densities of the BTs and PCTs used as photoanodes are mainly due to their better incident photons and photogenerated charge-harvesting capability compared to TNTAs resulting from their further enhanced and rough surface areas. As a result, our study will also provide a new approach in conformating hierarchical homogeneity nanostructure materials and presenting two kinds of promising candidates for applications in DSSCs, sensors, and photocatalysis.
branched TiO2 nanotube arrays
dye-sensitized solar cells
field-emission scanning electron microscopy
P25-coated TiO2 nanotube arrays
transmission electron microscopy
TiO2 nanotube arrays
Iijima S: Helical microtubules of graphitic carbon. Nature 1991, 354: 56. 10.1038/354056a0
Park S, Lim JH, Chung SW, Mirkin CA: Self-Assembly of Mesoscopic Metal-Polymer Amphiphiles. Science 2004, 303: 348. 10.1126/science.1093276
Chen XB, Mao SS: Titanium Dioxide Nanomaterials: Synthesis, Properties, Modific- ations, and Applications. Chem Rev 2007, 107: 2891. 10.1021/cr0500535
Zhang DF, Sun LD, Jia CJ, Yan ZG, You LP, Yan CH: Hierarchical Assembly of SnO 2 Nanorod Arrays on α-Fe 2 O 3 Nanotubes: A Case of Interfacial Lattice Compatibility. J Am Chem Soc 2005, 127: 13492. 10.1021/ja054771k
Cheng CW, Liu B, Yang HY, Zhou WW, Sun L, Chen R, Yu SF, Gong H, Zhang JX, Sun HD, Fan HJ: Hierarchical Assembly of ZnO Nanostructures on SnO 2 Backbone Nanowires: Low-Temperature Hydrothermal Preparation and Optical Properties. ACS Nano 2009, 3: 3069. 10.1021/nn900848x
Niu MT, Huang F, Cui LF, Huang P, Yu YL, Wang YS: Hydrothermal Synthesis, Structural Characteristics, and Enhanced Photocatalysis of SnO 2 /α-Fe 2 O 3 Semiconductor Nanoheterostructures. ACS Nano 2010, 4: 681. 10.1021/nn901119a
Oh YS, Lee JK, Kim HS, Han SB, Park KW: TiO 2 Branched Nanostructure Electrodes Synthesized by Seeding Method for Dye-Sensitized Solar Cells. Chem Mater 2010, 22: 1114. 10.1021/cm902272q
Wang J, Lin J: Freestanding TiO 2 Nanotube Arrays with Ultrahigh Aspect Ratio via Electrochemical Anodization. Chem Mater 2008, 20: 1257. 10.1021/cm7028917
Mor GK, Shankar K, Paulose M, Varghese OK, Grimes CA: Use of Highly-Ordered TiO 2 Nanotube Arrays in Dye-Sensitized Solar Cells. Nano Lett 2006, 6: 215. 10.1021/nl052099j
Albu SP, Ghicov A, Aldabergenova S, Drechsel P, LeClere D, Thompson GE, Macak JM, Schmuki P: Formation of Double-Walled TiO 2 Nanotubes and Robust Anatase Membranes Communication. Adv Mater 2008, 20: 4135.
Mor GK, Shankar K, Paulose M, Varghese OK, Grimes CA: Enhanced Photocleavage of Water Using Titania Nanotube Arrays. Nano Lett 2005, 5: 191. 10.1021/nl048301k
Liu L, Qian JS, Li B, Cui B, Zhou XF, Guo XF, Ding WP: Fabrication of rutile TiO 2 tapered nanotubes with rectangular cross-sections via anisotropic corrosion route. Chem Commun 2010, 46: 2402. 10.1039/b921750a
Yoriya S, Grimes CA: Self-Assembled TiO 2 Nanotube Arrays by Anodization of Titanium in Diethylene Glycol: Approach to Extended Pore Widening. Langmuir 2010, 26: 417. 10.1021/la9020146
Kim D, Ghicov A, Albu SP, Schmuki P: Bamboo-Type TiO 2 Nanotubes: Improved Conversion Efficiency in Dye-Sensitized Solar Cells. J Am Chem Soc 2008, 130: 16454. 10.1021/ja805201v
Kang SH, Kim JY, Kim Y, Kim HS, Sung YE: Surface Modification of Stretched TiO 2 Nanotubes for Solid-State Dye-Sensitized Solar Cells. J Phys Chem C 2007, 111: 9614. 10.1021/jp071504n
Wang DA, Liu Y, Wang CW, Zhou F, Liu WM: Highly Flexible Coaxial Nanohybrids Made from Porous TiO 2 Nanotubes. ACS Nano 2009, 3: 1249. 10.1021/nn900154z
Wang DA, Hu TC, Hu LT, Yu B, Xia YQ, Zhou F, Liu WM: Microstructured Arrays of TiO 2 Nanotubes for Improved Photo-Electrocatalysis and Mechanical Stability. Adv Funct Mater 2009, 19: 1930. 10.1002/adfm.200801703
Meng S, Ren J, Kaxiras E: Natural Dyes Adsorbed on TiO 2 Nanowire for Photovoltaic Applications: Enhanced Light Absorption and Ultrafast Electron Injection. Nano Lett 2008, 8: 3266. 10.1021/nl801644d
Paulose M, Shankar K, Varghese OK, Mor GK, Hardin B, Grimes CA: Backside illuminated dye-sensitized solar cells based on titania nanotube array electrodes. Nanotechnology 2006, 17: 1446. 10.1088/0957-4484/17/5/046
Mohapatra SK, Misra M: Enhanced Photoelectrochemical Generation of Hydrogen from Water by 2,6-Dihydroxyantraquinone-Functionalized Titanium Dioxide Nanotubes. J Phys Chem C 2007, 111: 11506. 10.1021/jp0728712
Mor GK, Prakasam HE, Varghese OK, Shankar K, Grimes CA: Vertically Oriented Ti-Fe-O Nanotube Array Films: Toward a Useful Material Architecture for Solar Spectrum Water Photoelectrolysis. Nano Lett 2007, 7: 2356. (2007) (2007) 10.1021/nl0710046
Zheng Q, Zhou Q, Bai J, Li LH, Jin ZJ, Zhang JL, Li JH, Liu YB, Cai WM, Zhu XY: Self-Organized TiO 2 Nanotube Array Sensor for the Determination of Chemical Oxygen Demand. Adv Mater 2008, 20: 1044. 10.1002/adma.200701619
Fang XS, Bando Y, Gautam UK, Ye CH, Golberg D: Inorganic semiconductor nanostructures and their field-emission Applications. J Mater Chem 2008, 18: 509. 10.1039/b712874f
Shin K, Seok SI, Im SH, Park JH: CdS or CdSe decorated TiO 2 nanotube arrays from spray pyrolysis deposition: use in photoelectrochemical cells. Chem Commun 2010, 46: 2385. 10.1039/b923022j
Macak JM, Zollfrank C, Rodriguez BJ, Tsuchiya H, Alexe M, Greil P, Schmuki P: Ordered Ferroelectric Lead Titanate Nanocellular Structure by Conversion of Anodic TiO 2 Nanotubes. Adv Mater 2009, 21: 3121. 10.1002/adma.200900587
Albu SP, Ghicov A, Macak A, Hahn R, Schmuki P: Self-Organized, Free-Standing TiO 2 Nanotube Membrane for Flow-through Photocatalytic Applications. Nano Lett 2007, 7: 1286. 10.1021/nl070264k
Roy P, Kim D, Lee K, Spiecker E, Schmuki P: TiO 2 nanotubes and their application in dye-sensitized solar cells. Nanoscale 2010, 2: 45. 10.1039/b9nr00131j
Wang J, Zhao L, Lin VSY, Lin ZQ: Formation of various TiO 2 nanostructures from electrochemically anodized titanium. J Mater Chem 2009, 19: 3682. 10.1039/b904247d
Varghese OK, Gong OK, Paulose M, Grimes CA, Dickey EC: Crystallization and high-temperature structural stability of titanium oxide nanotube arrays. J Mater Res 2003, 18: 156. 10.1557/JMR.2003.0022
Macak JM, Gong BG, Hueppe M, Schmuki P: Filling of TiO 2 Nanotubes by Self-Doping and Electrodeposition. Adv Mater 2007, 19: 3027. 10.1002/adma.200602549
Woan K, Pyrgiotakis G, Sigmund W: Photocatalytic Carbon-Nanotube- TiO 2 Composites. Adv Mater 2009, 21: 2233. 10.1002/adma.200802738
Wang DA, Yu B, Wang CW, Zhou F, Liu WM: A Novel Protocol Towards Perfect Alignment of Defect-Free Anodized TiO 2 Nanotubes. Adv Mater 2009, 21: 1964. 10.1002/adma.200801996
Lin YJ, Zhou S, Liu XH, Sheehan S, Wang DW: TiO 2 /TiSi 2 Heterostructures for High-Efficiency Photoelectrochemical H 2 O Splitting. J Am Chem Soc 2009, 131: 2772. 10.1021/ja808426h
Cheng HM, Chiu WH, Lee CH, Tsai SY, Hsieh WF: Formation of Branched ZnO Nanowires from Solvothermal Method and Dye-Sensitized Solar Cells Applications. J Phys Chem C 2008, 112: 16359. 10.1021/jp805239k
Roy P, Kim D, Paramasivam I, Schmuki P: Improved efficiency of TiO 2 nanotubes in dye sensitized solar cells by decoration with TiO 2 nanoparticles. Electrochem Commun 2009, 11: 1001. 10.1016/j.elecom.2009.02.049
Prakasam HE, Shankar K, Paulose M, Varghese OK, Grimes CA: A New Benchmark for TiO 2 Nanotube Array Growth by Anodization. J Phys Chem C 2007, 111: 7235. 10.1021/jp070273h
Shankar K, Bandara J, Paulose M, Wietasch H, Varghese OK, Mor GK, LaTempa TJ, Thelakkat M, Grimes CA: Highly Efficient Solar Cells using TiO 2 Nanotube Arrays Sensitized with a Donor-Antenna Dye. Nano Lett 2008, 8: 1654. 10.1021/nl080421v
Xiao XF, Ouyang K, Liu RF, Liang JH: Anatase type titania nanotube arrays direct fabricated by anodization without annealing. Appl Surf Sci 2009, 255: 3659. 10.1016/j.apsusc.2008.10.014
Pan JH, Zhang X, Du AJ, Sun DD, Leckie JO: Self-Etching Reconstruction of Hierarchically Mesoporous F-TiO 2 Hollow Microspherical Photocatalyst for Concurrent Membrane Water Purifications. J Am Chem Soc 2008, 130: 11256. 10.1021/ja803582m
Zuo F, Wang L, Wu T, Zhang ZY, Borchardt D, Feng PY: Self-Doped Ti 3+ Enhanced Photocatalyst for Hydrogen Production under Visible Light. J Am Chem Soc 2010, 132: 11856. 10.1021/ja103843d
Zhou JK, Lv L, Yu J, Li HL, Guo PZ, Sun H, Zhao XS: Synthesis of Self-Organized Polycrystalline F-doped TiO 2 Hollow Microspheres and Their Photocatalytic Activity under Visible Light. J Phys Chem C 2008, 112: 5316. 10.1021/jp709615x
Dong X, Tao J, Li YY, Zhu H: Enhanced photoelectrochemical properties of F-containing TiO 2 sphere thin film induced by its novel hierarchical structure. Appl Surf Sci 2009, 255: 7183. 10.1016/j.apsusc.2009.03.056
Park JH, Kim S, Bard AJ: Novel Carbon-Doped TiO 2 Nanotube Arrays with High Aspect Ratios for Efficient Solar Water Splitting. Nano Lett 2006, 6: 24. 10.1021/nl051807y
Marin FI, Hamstra MA, Vanmaekelbergh D: Greatly Enhanced Sub-Bandgap Photocurrent in Porous GaP Photoanodes. J Electrochem Soc 1996, 143: 1137. 10.1149/1.1836597
The authors would like to acknowledge financial support for this study from the National Natural Science Foundation of China (No. 50872039; 50802032), and the Xiangyang Plans Projects of Scientific and Technological Research and Development (No. 2010GG1B35).
The authors declare that they have no competing interests.
AH presided over and fully participated in all of the work. CC and XL participated in the preparation of the samples. JJ and RM participated in the revision of the manuscript and the statistical analysis of experimental data. JH and FW participated in the investigation of the photocurrent performances. XT and JP participated in the design and idea of the study. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.